#------------------------------------------------------------------------------
#$Date: 2017-11-04 02:13:38 +0200 (Sat, 04 Nov 2017) $
#$Revision: 202561 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/12/66/4126674.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4126674
loop_
_publ_author_name
'Qin, Lei'
'Zhou, Guojun'
'Yu, You-Zhu'
'Nojiri, Hiroyuki'
'Schröder, Christian'
'Winpenny, Richard E. P.'
'Zheng, Yan-Zhen'
_publ_section_title
;
 Topological Self-Assembly of Highly-Symmetric Lanthanide Clusters: A
 Magnetic Study of Exchange-Coupling "Fingerprints" in Giant
 Gadolinium(III) Cages.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.7b09996
_journal_year                    2017
_chemical_formula_sum            'C50 H130 Cl Gd15 O70'
_chemical_formula_weight         4245.73
_chemical_name_common            Gd15
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           20
_space_group_name_Hall           'C 2c 2'
_space_group_name_H-M_alt        'C 2 2 21'
_symmetry_space_group_name_Hall  'C 2c 2'
_symmetry_space_group_name_H-M   'C 2 2 21'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   20.230(2)
_cell_length_b                   30.537(3)
_cell_length_c                   28.675(3)
_cell_measurement_reflns_used    9525
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.46
_cell_measurement_theta_min      2.24
_cell_volume                     17714(3)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0267
_diffrn_reflns_av_unetI/netI     0.0353
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       36
_diffrn_reflns_limit_k_min       -39
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_limit_l_min       -36
_diffrn_reflns_number            63791
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.542
_diffrn_reflns_theta_min         1.401
_exptl_absorpt_coefficient_mu    5.603
_exptl_absorpt_correction_T_max  0.218
_exptl_absorpt_correction_T_min  0.148
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.592
_exptl_crystal_description       octahedron
_exptl_crystal_F_000             7868
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.32
_exptl_crystal_size_min          0.26
_platon_squeeze_details
;
;
_refine_diff_density_max         5.454
_refine_diff_density_min         -4.102
_refine_diff_density_rms         0.280
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.73(3)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.090
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     573
_refine_ls_number_reflns         20250
_refine_ls_number_restraints     1410
_refine_ls_restrained_S_all      1.079
_refine_ls_R_factor_all          0.0647
_refine_ls_R_factor_gt           0.0554
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0860P)²+319.5692P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1481
_refine_ls_wR_factor_ref         0.1563
_reflns_Friedel_coverage         0.876
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.994
_reflns_number_gt                17631
_reflns_number_total             20250
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ja7b09996_si_002.cif
_cod_data_source_block           Gd15
_cod_database_code               4126674
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014-3
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
C1 C 1.1533(11) 0.0702(7) 0.7629(8) 0.0520(16) Uani 1 1 d . U .
C2 C 1.2038(11) 0.0404(7) 0.7384(7) 0.0520(16) Uani 1 1 d . U .
C3 C 1.1734(11) 0.0057(7) 0.7139(8) 0.0520(16) Uani 1 1 d . U .
H3A H 1.1530 -0.0121 0.7374 0.062 Uiso 1 1 d R U .
H3C H 1.2080 -0.0116 0.7004 0.062 Uiso 1 1 d R U .
C4 C 1.2516(11) 0.0652(8) 0.7068(8) 0.055(3) Uani 1 1 d . U .
H4A H 1.2769 0.0870 0.7252 0.066 Uiso 1 1 calc R U .
H4B H 1.2833 0.0446 0.6923 0.066 Uiso 1 1 calc R U .
C5 C 1.2531(13) 0.0213(9) 0.7801(10) 0.069(5) Uani 1 1 d . U .
H5A H 1.2737 0.0459 0.7966 0.104 Uiso 1 1 calc R U .
H5B H 1.2272 0.0038 0.8021 0.104 Uiso 1 1 calc R U .
H5C H 1.2876 0.0030 0.7661 0.104 Uiso 1 1 calc R U .
C6 C 1.1504(9) 0.1753(6) 0.5843(6) 0.033(2) Uani 1 1 d . U .
C7 C 1.2021(10) 0.1891(6) 0.5475(7) 0.039(3) Uani 1 1 d . U .
C8 C 1.1669(10) 0.2017(6) 0.5007(7) 0.041(3) Uani 1 1 d . U .
H8A H 1.2003 0.2047 0.4757 0.049 Uiso 1 1 calc R U .
H8C H 1.1357 0.1782 0.4917 0.049 Uiso 1 1 calc R U .
C9 C 1.2475(9) 0.2249(6) 0.5717(7) 0.042(3) Uani 1 1 d . U .
H9A H 1.2682 0.2121 0.5999 0.050 Uiso 1 1 calc R U .
H9B H 1.2833 0.2334 0.5500 0.050 Uiso 1 1 calc R U .
C10 C 1.2491(10) 0.1483(7) 0.5350(7) 0.047(4) Uani 1 1 d . U .
H10A H 1.2817 0.1573 0.5116 0.071 Uiso 1 1 calc R U .
H10B H 1.2719 0.1384 0.5632 0.071 Uiso 1 1 calc R U .
H10C H 1.2223 0.1243 0.5225 0.071 Uiso 1 1 calc R U .
C11 C 0.8543(8) 0.1914(5) 0.5725(6) 0.032(2) Uani 1 1 d . U .
C12 C 0.8053(9) 0.1573(6) 0.5491(7) 0.039(3) Uani 1 1 d . U .
C13 C 0.7620(9) 0.1389(6) 0.5859(7) 0.042(3) Uani 1 1 d . U .
H13A H 0.7343 0.1171 0.5718 0.050 Uiso 1 1 d R U .
H13D H 0.7336 0.1616 0.5975 0.050 Uiso 1 1 d R U .
C14 C 0.8419(10) 0.1216(6) 0.5251(7) 0.039(3) Uani 1 1 d . U .
H14A H 0.8702 0.1346 0.5021 0.047 Uiso 1 1 d R U .
H14B H 0.8099 0.1042 0.5086 0.047 Uiso 1 1 d R U .
C15 C 0.7665(10) 0.1798(7) 0.5101(8) 0.046(4) Uani 1 1 d . U .
H15A H 0.7974 0.1914 0.4868 0.069 Uiso 1 1 calc R U .
H15B H 0.7368 0.1586 0.4953 0.069 Uiso 1 1 calc R U .
H15C H 0.7405 0.2040 0.5232 0.069 Uiso 1 1 calc R U .
C16 C 0.8479(8) 0.3747(5) 0.6524(5) 0.026(2) Uani 1 1 d . U .
C17 C 0.7962(8) 0.3832(5) 0.6141(5) 0.031(3) Uani 1 1 d . U .
C18 C 0.7536(9) 0.3441(6) 0.6076(6) 0.033(3) Uani 1 1 d . U .
H18A H 0.7305 0.3377 0.6373 0.040 Uiso 1 1 calc R U .
H18B H 0.7196 0.3507 0.5838 0.040 Uiso 1 1 calc R U .
C19 C 0.8321(9) 0.3987(6) 0.5700(6) 0.034(3) Uani 1 1 d . U .
H19A H 0.7985 0.4085 0.5472 0.041 Uiso 1 1 calc R U .
H19B H 0.8595 0.4244 0.5782 0.041 Uiso 1 1 calc R U .
C20 C 0.7501(9) 0.4219(6) 0.6282(6) 0.038(3) Uani 1 1 d . U .
H20A H 0.7766 0.4484 0.6328 0.056 Uiso 1 1 calc R U .
H20B H 0.7176 0.4270 0.6035 0.056 Uiso 1 1 calc R U .
H20C H 0.7271 0.4146 0.6573 0.056 Uiso 1 1 calc R U .
C21 C 0.7515(8) 0.3945(6) 0.8187(6) 0.032(3) Uani 1 1 d . U .
H21A H 0.7289 0.3659 0.8217 0.039 Uiso 1 1 calc R U .
H21B H 0.7175 0.4178 0.8184 0.039 Uiso 1 1 calc R U .
C22 C 0.7994(8) 0.4014(5) 0.8617(6) 0.033(3) Uani 1 1 d . U .
C23 C 0.8519(8) 0.3655(5) 0.8647(5) 0.027(2) Uani 1 1 d . U .
C24 C 0.8339(8) 0.4480(5) 0.8621(6) 0.029(2) Uani 1 1 d . U .
H24A H 0.7994 0.4710 0.8632 0.035 Uiso 1 1 calc R U .
H24B H 0.8613 0.4508 0.8906 0.035 Uiso 1 1 calc R U .
C25 C 0.7521(9) 0.4019(6) 0.9054(6) 0.040(4) Uani 1 1 d . U .
H25A H 0.7195 0.4255 0.9019 0.060 Uiso 1 1 calc R U .
H25B H 0.7292 0.3737 0.9078 0.060 Uiso 1 1 calc R U .
H25C H 0.7781 0.4070 0.9338 0.060 Uiso 1 1 calc R U .
Cl1 Cl 1.0000 0.23503(11) 0.7500 0.0106(6) Uani 1 2 d S T P
Gd1 Gd 1.0000 0.13174(3) 0.7500 0.0298(2) Uani 1 2 d S T P
Gd2 Gd 0.90804(5) 0.10005(3) 0.63461(3) 0.0372(2) Uani 1 1 d . . .
Gd3 Gd 1.09462(5) 0.08897(3) 0.65019(3) 0.03548(19) Uani 1 1 d D . .
Gd4 Gd 1.00168(4) 0.20065(2) 0.63890(2) 0.02503(11) Uani 1 1 d . . .
Gd5 Gd 1.09652(4) 0.27994(2) 0.57395(2) 0.02503(11) Uani 1 1 d . . .
Gd6 Gd 1.00012(5) 0.31998(2) 0.68326(2) 0.02503(11) Uani 1 1 d . . .
Gd7 Gd 0.90630(5) 0.29563(2) 0.57809(3) 0.03077(18) Uani 1 1 d . . .
Gd8 Gd 0.90540(4) 0.40553(2) 0.75903(2) 0.02509(16) Uani 1 1 d . . .
O1 O 1.0697(5) 0.1589(3) 0.6877(3) 0.0194(16) Uani 1 1 d . U .
H1A H 1.1098 0.1749 0.6990 0.023 Uiso 1 1 calc R U .
O2 O 0.9920(5) 0.0794(3) 0.6893(3) 0.0236(18) Uani 1 1 d . U .
H2A H 0.9859 0.0490 0.7013 0.028 Uiso 1 1 calc R U .
O3 O 0.9310(5) 0.1575(3) 0.6892(3) 0.0162(16) Uani 1 1 d . U .
H3B H 0.8908 0.1734 0.7003 0.019 Uiso 1 1 calc R U .
O4 O 1.0089(6) 0.1271(3) 0.6089(3) 0.0248(17) Uani 1 1 d . U .
H4C H 1.0141 0.1259 0.5743 0.030 Uiso 1 1 calc R U .
O5 O 0.9321(5) 0.2628(3) 0.6516(3) 0.0164(15) Uani 1 1 d . U .
H5D H 0.8923 0.2562 0.6710 0.020 Uiso 1 1 calc R U .
O6 O 1.0696(5) 0.2632(4) 0.6523(4) 0.02503(11) Uani 1 1 d . U .
H6A H 1.1091 0.2568 0.6721 0.030 Uiso 1 1 calc R U .
O7 O 0.9933(5) 0.2442(3) 0.5675(3) 0.0203(16) Uani 1 1 d . U .
H7A H 0.9887 0.2261 0.5386 0.024 Uiso 1 1 calc R U .
O8 O 1.0083(5) 0.3273(3) 0.5994(3) 0.0147(16) Uani 1 1 d . U .
H8B H 1.0134 0.3583 0.5887 0.018 Uiso 1 1 calc R U .
O9 O 0.9302(4) 0.3290(3) 0.7495(3) 0.0136(14) Uani 1 1 d . U .
H9C H 0.8903 0.3096 0.7494 0.016 Uiso 1 1 calc R U .
O10 O 1.1103(6) 0.0877(4) 0.7352(4) 0.035(2) Uani 1 1 d . U .
O11 O 1.2117(6) 0.0879(5) 0.6697(5) 0.043(2) Uani 1 1 d . U .
H11A H 1.2351 0.1040 0.6521 0.052 Uiso 1 1 d R U .
O12 O 1.1204(8) 0.0144(5) 0.6749(5) 0.0520(16) Uani 1 1 d . U .
H12A H 1.1004 -0.0072 0.6624 0.062 Uiso 1 1 d R U .
O13 O 1.0528(6) 0.0286(3) 0.6161(4) 0.03548(19) Uani 1 1 d D U .
H90B H 1.0095 0.0228 0.6284 0.053 Uiso 1 1 d R U .
H90C H 1.0497 0.0334 0.5831 0.053 Uiso 1 1 d R U .
O14 O 1.1427(9) 0.0540(5) 0.5825(6) 0.061(4) Uani 1 1 d . U .
H91A H 1.1632 0.0271 0.5921 0.092 Uiso 1 1 d R U .
H91C H 1.1754 0.0730 0.5690 0.092 Uiso 1 1 d R U .
O15 O 1.1575(5) 0.1388(3) 0.6049(4) 0.0244(18) Uani 1 1 d . U .
O16 O 1.1044(5) 0.2013(3) 0.5913(3) 0.0245(17) Uani 1 1 d . U .
O17 O 1.1327(6) 0.2411(4) 0.5058(4) 0.034(2) Uani 1 1 d . U .
H17A H 1.1234 0.2538 0.4803 0.041 Uiso 1 1 d R U .
O18 O 1.2130(5) 0.2610(4) 0.5841(4) 0.030(2) Uani 1 1 d . U .
H18C H 1.2360 0.2805 0.5977 0.036 Uiso 1 1 d R U .
O19 O 0.8479(6) 0.3406(4) 0.8980(4) 0.029(2) Uani 1 1 d . U .
O20 O 1.0806(8) 0.3257(5) 0.5083(5) 0.056(3) Uani 1 1 d . U .
H20E H 1.0398 0.3262 0.5013 0.084 Uiso 1 1 d R U .
H20F H 1.0936 0.3515 0.5144 0.084 Uiso 1 1 d R U .
O22 O 1.1528(6) 0.0729(4) 0.8036(5) 0.041(3) Uani 1 1 d . U .
O23 O 0.7934(7) 0.1203(4) 0.6221(5) 0.044(2) Uani 1 1 d . U .
H23A H 0.7683 0.1145 0.6450 0.053 Uiso 1 1 d R U .
O24 O 0.8806(7) 0.0923(5) 0.5537(5) 0.049(3) Uani 1 1 d . U .
H24C H 0.8963 0.0700 0.5398 0.059 Uiso 1 1 d R U .
O25 O 0.8985(6) 0.1737(3) 0.5980(3) 0.0273(17) Uani 1 1 d . U .
O26 O 0.8485(6) 0.2291(4) 0.5644(4) 0.030(2) Uani 1 1 d . U .
O27 O 0.9218(9) 0.2957(5) 0.4955(5) 0.063(4) Uani 1 1 d . U .
H27A H 0.9002 0.3169 0.4837 0.094 Uiso 1 1 d R U .
H27C H 0.9078 0.2717 0.4842 0.094 Uiso 1 1 d R U .
O28 O 0.8731(6) 0.3673(3) 0.5481(4) 0.0271(19) Uani 1 1 d . U .
H28A H 0.8880 0.3742 0.5214 0.032 Uiso 1 1 d R U .
O29 O 0.7900(5) 0.3063(4) 0.5934(4) 0.0271(19) Uani 1 1 d . U .
H29A H 0.7665 0.2834 0.5899 0.033 Uiso 1 1 d R U .
O30 O 0.8932(5) 0.3473(3) 0.6438(3) 0.0225(17) Uani 1 1 d . U .
O31 O 0.8471(5) 0.3951(3) 0.6902(3) 0.0235(18) Uani 1 1 d . U .
O32 O 0.8746(6) 0.4548(4) 0.8220(4) 0.032(2) Uani 1 1 d . U .
H32A H 0.8914 0.4802 0.8200 0.038 Uiso 1 1 d R U .
O33 O 0.7876(5) 0.3956(4) 0.7768(4) 0.030(2) Uani 1 1 d . U .
H33A H 0.7638 0.3918 0.7527 0.035 Uiso 1 1 d R U .
O34 O 0.8926(5) 0.3638(3) 0.8324(3) 0.0195(17) Uani 1 1 d . U .
O35 O 0.9190(9) 0.4783(4) 0.7310(5) 0.056(4) Uani 1 1 d . U .
H35A H 0.8976 0.4957 0.7485 0.083 Uiso 1 1 d R U .
H35C H 0.9041 0.4799 0.7033 0.083 Uiso 1 1 d R U .
O36 O 1.0071(5) 0.3963(3) 0.7976(3) 0.0141(16) Uani 1 1 d . U .
H10G H 1.0122 0.4156 0.8255 0.017 Uiso 1 1 calc R U .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O22 C1 O10 125.3(19) . .
O22 C1 C2 120.2(19) . .
O10 C1 C2 114.2(18) . .
C3 C2 C4 110.7(19) . .
C3 C2 C1 112(2) . .
C4 C2 C1 113.6(18) . .
C3 C2 C5 110.8(18) . .
C4 C2 C5 102.7(18) . .
C1 C2 C5 106.1(18) . .
C2 C3 O12 121.6(18) . .
O11 C4 C2 107.9(17) . .
O16 C6 O15 124.9(14) . .
O16 C6 C7 116.4(15) . .
O15 C6 C7 118.7(14) . .
C6 C7 C8 110.2(16) . .
C6 C7 C9 106.3(14) . .
C8 C7 C9 117.9(16) . .
C6 C7 C10 110.0(14) . .
C8 C7 C10 105.6(15) . .
C9 C7 C10 106.8(16) . .
O17 C8 C7 110.4(15) . .
O18 C9 C7 112.2(15) . .
O26 C11 O25 126.6(15) . .
O26 C11 C12 119.6(15) . .
O25 C11 C12 113.7(14) . .
C13 C12 C14 110.2(17) . .
C13 C12 C15 112.8(16) . .
C14 C12 C15 104.2(16) . .
C13 C12 C11 108.4(15) . .
C14 C12 C11 111.6(15) . .
C15 C12 C11 109.5(15) . .
O23 C13 C12 115.5(16) . .
O24 C14 C12 117.4(16) . .
O31 C16 O30 120.5(14) . .
O31 C16 C17 121.8(13) . .
O30 C16 C17 117.6(12) . .
C18 C17 C19 114.9(13) . .
C18 C17 C16 110.4(14) . .
C19 C17 C16 108.7(14) . .
C18 C17 C20 107.1(14) . .
C19 C17 C20 105.3(14) . .
C16 C17 C20 110.4(12) . .
O29 C18 C17 112.7(14) . .
O28 C19 C17 115.7(14) . .
O33 C21 C22 110.2(13) . .
C23 C22 C25 112.6(13) . .
C23 C22 C24 109.8(14) . .
C25 C22 C24 104.7(14) . .
C23 C22 C21 111.8(14) . .
C25 C22 C21 104.4(14) . .
C24 C22 C21 113.3(13) . .
O19 C23 O34 126.9(14) . .
O19 C23 C22 116.4(13) . .
O34 C23 C22 116.7(13) . .
O32 C24 C22 112.2(12) . .
Gd1 Cl1 Gd6 143.58(4) . 3_756
Gd1 Cl1 Gd6 143.58(4) . .
Gd6 Cl1 Gd6 72.84(8) 3_756 .
O3 Gd1 O3 141.2(4) 3_756 .
O3 Gd1 O2 69.0(3) 3_756 3_756
O3 Gd1 O2 143.7(3) . 3_756
O3 Gd1 O2 143.7(3) 3_756 .
O3 Gd1 O2 69.0(3) . .
O2 Gd1 O2 95.2(4) 3_756 .
O3 Gd1 O1 71.7(3) 3_756 3_756
O3 Gd1 O1 94.9(3) . 3_756
O2 Gd1 O1 74.2(3) 3_756 3_756
O2 Gd1 O1 137.1(3) . 3_756
O3 Gd1 O1 94.9(3) 3_756 .
O3 Gd1 O1 71.7(3) . .
O2 Gd1 O1 137.1(3) 3_756 .
O2 Gd1 O1 74.2(3) . .
O1 Gd1 O1 140.0(5) 3_756 .
O3 Gd1 O10 123.3(3) 3_756 3_756
O3 Gd1 O10 77.8(3) . 3_756
O2 Gd1 O10 66.2(4) 3_756 3_756
O2 Gd1 O10 73.5(3) . 3_756
O1 Gd1 O10 64.1(3) 3_756 3_756
O1 Gd1 O10 141.7(3) . 3_756
O3 Gd1 O10 77.8(3) 3_756 .
O3 Gd1 O10 123.3(3) . .
O2 Gd1 O10 73.5(3) 3_756 .
O2 Gd1 O10 66.2(4) . .
O1 Gd1 O10 141.7(3) 3_756 .
O1 Gd1 O10 64.1(3) . .
O10 Gd1 O10 118.8(5) 3_756 .
O3 Gd1 Cl1 70.6(2) 3_756 .
O3 Gd1 Cl1 70.6(2) . .
O2 Gd1 Cl1 132.4(2) 3_756 .
O2 Gd1 Cl1 132.4(2) . .
O1 Gd1 Cl1 70.0(2) 3_756 .
O1 Gd1 Cl1 70.0(2) . .
O10 Gd1 Cl1 120.6(3) 3_756 .
O10 Gd1 Cl1 120.6(3) . .
O3 Gd1 Gd3 81.5(2) 3_756 3_756
O3 Gd1 Gd3 112.6(2) . 3_756
O2 Gd1 Gd3 39.2(3) 3_756 3_756
O2 Gd1 Gd3 107.3(2) . 3_756
O1 Gd1 Gd3 41.0(2) 3_756 3_756
O1 Gd1 Gd3 175.7(2) . 3_756
O10 Gd1 Gd3 41.9(2) 3_756 3_756
O10 Gd1 Gd3 112.6(2) . 3_756
Cl1 Gd1 Gd3 110.77(2) . 3_756
O3 Gd1 Gd3 112.6(2) 3_756 .
O3 Gd1 Gd3 81.5(2) . .
O2 Gd1 Gd3 107.3(2) 3_756 .
O2 Gd1 Gd3 39.2(3) . .
O1 Gd1 Gd3 175.7(2) 3_756 .
O1 Gd1 Gd3 41.0(2) . .
O10 Gd1 Gd3 112.5(2) 3_756 .
O10 Gd1 Gd3 41.9(2) . .
Cl1 Gd1 Gd3 110.77(2) . .
Gd3 Gd1 Gd3 138.46(4) 3_756 .
O3 Gd1 Gd4 115.2(2) 3_756 .
O3 Gd1 Gd4 37.6(2) . .
O2 Gd1 Gd4 169.9(2) 3_756 .
O2 Gd1 Gd4 76.0(2) . .
O1 Gd1 Gd4 115.6(2) 3_756 .
O1 Gd1 Gd4 36.0(2) . .
O10 Gd1 Gd4 115.0(3) 3_756 .
O10 Gd1 Gd4 98.0(2) . .
Cl1 Gd1 Gd4 56.556(17) . .
Gd3 Gd1 Gd4 148.05(2) 3_756 .
Gd3 Gd1 Gd4 62.765(18) . .
O22 Gd2 O4 147.0(4) 3_756 .
O22 Gd2 O2 77.4(4) 3_756 .
O4 Gd2 O2 71.2(4) . .
O22 Gd2 O3 82.3(4) 3_756 .
O4 Gd2 O3 77.0(3) . .
O2 Gd2 O3 68.2(3) . .
O22 Gd2 O24 125.7(5) 3_756 .
O4 Gd2 O24 86.1(4) . .
O2 Gd2 O24 140.5(4) . .
O3 Gd2 O24 138.5(4) . .
O22 Gd2 O23 72.3(5) 3_756 .
O4 Gd2 O23 134.6(4) . .
O2 Gd2 O23 147.3(4) . .
O3 Gd2 O23 95.5(4) . .
O24 Gd2 O23 70.1(5) . .
O22 Gd2 O25 127.3(4) 3_756 .
O4 Gd2 O25 67.2(4) . .
O2 Gd2 O25 124.6(4) . .
O3 Gd2 O25 68.2(3) . .
O24 Gd2 O25 70.3(4) . .
O23 Gd2 O25 68.5(4) . .
O22 Gd2 Gd4 123.9(3) 3_756 .
O4 Gd2 Gd4 41.1(2) . .
O2 Gd2 Gd4 80.2(2) . .
O3 Gd2 Gd4 41.7(2) . .
O24 Gd2 Gd4 103.8(4) . .
O23 Gd2 Gd4 106.8(3) . .
O25 Gd2 Gd4 44.5(2) . .
O22 Gd2 Gd3 113.9(3) 3_756 .
O4 Gd2 Gd3 36.8(3) . .
O2 Gd2 Gd3 36.7(2) . .
O3 Gd2 Gd3 78.3(2) . .
O24 Gd2 Gd3 109.5(4) . .
O23 Gd2 Gd3 170.1(3) . .
O25 Gd2 Gd3 101.9(3) . .
Gd4 Gd2 Gd3 63.42(2) . .
O22 Gd2 Gd1 72.2(3) 3_756 .
O4 Gd2 Gd1 76.3(2) . .
O2 Gd2 Gd1 34.5(2) . .
O3 Gd2 Gd1 34.5(2) . .
O24 Gd2 Gd1 162.1(4) . .
O23 Gd2 Gd1 121.1(4) . .
O25 Gd2 Gd1 99.8(2) . .
Gd4 Gd2 Gd1 60.79(2) . .
Gd3 Gd2 Gd1 56.858(19) . .
O13 Gd3 O15 119.3(4) . .
O13 Gd3 O2 77.1(4) . .
O15 Gd3 O2 143.7(3) . .
O13 Gd3 O4 84.9(4) . .
O15 Gd3 O4 78.8(4) . .
O2 Gd3 O4 70.2(3) . .
O13 Gd3 O14 56.1(5) . .
O15 Gd3 O14 68.1(4) . .
O2 Gd3 O14 132.5(5) . .
O4 Gd3 O14 96.3(5) . .
O13 Gd3 O11 117.0(5) . .
O15 Gd3 O11 67.2(4) . .
O2 Gd3 O11 137.7(4) . .
O4 Gd3 O11 145.4(4) . .
O14 Gd3 O11 77.7(6) . .
O13 Gd3 O12 56.1(5) . .
O15 Gd3 O12 130.0(4) . .
O2 Gd3 O12 86.3(4) . .
O4 Gd3 O12 138.6(5) . .
O14 Gd3 O12 74.6(5) . .
O11 Gd3 O12 73.3(5) . .
O13 Gd3 O1 146.0(4) . .
O15 Gd3 O1 78.0(3) . .
O2 Gd3 O1 73.7(3) . .
O4 Gd3 O1 69.2(3) . .
O14 Gd3 O1 145.3(4) . .
O11 Gd3 O1 96.4(4) . .
O12 Gd3 O1 137.0(4) . .
O13 Gd3 O10 117.8(4) . .
O15 Gd3 O10 119.0(4) . .
O2 Gd3 O10 69.1(4) . .
O4 Gd3 O10 126.1(3) . .
O14 Gd3 O10 137.4(5) . .
O11 Gd3 O10 69.3(4) . .
O12 Gd3 O10 70.8(4) . .
O1 Gd3 O10 66.6(3) . .
O13 Gd3 Gd1 115.6(3) . .
O15 Gd3 Gd1 118.5(2) . .
O2 Gd3 Gd1 39.0(2) . .
O4 Gd3 Gd1 80.5(2) . .
O14 Gd3 Gd1 171.5(4) . .
O11 Gd3 Gd1 109.4(3) . .
O12 Gd3 Gd1 102.5(3) . .
O1 Gd3 Gd1 40.6(2) . .
O10 Gd3 Gd1 45.7(3) . .
O13 Gd3 Gd2 69.5(3) . .
O15 Gd3 Gd2 114.2(3) . .
O2 Gd3 Gd2 37.1(2) . .
O4 Gd3 Gd2 35.4(3) . .
O14 Gd3 Gd2 110.1(5) . .
O11 Gd3 Gd2 172.2(3) . .
O12 Gd3 Gd2 109.1(4) . .
O1 Gd3 Gd2 76.7(2) . .
O10 Gd3 Gd2 104.2(3) . .
Gd1 Gd3 Gd2 62.96(2) . .
O13 Gd3 Gd4 119.8(3) . .
O15 Gd3 Gd4 69.7(2) . .
O2 Gd3 Gd4 74.1(2) . .
O4 Gd3 Gd4 35.7(2) . .
O14 Gd3 Gd4 120.8(4) . .
O11 Gd3 Gd4 119.9(3) . .
O12 Gd3 Gd4 160.2(3) . .
O1 Gd3 Gd4 34.4(2) . .
O10 Gd3 Gd4 99.1(3) . .
Gd1 Gd3 Gd4 60.32(2) . .
Gd2 Gd3 Gd4 55.73(2) . .
O1 Gd4 O6 90.1(4) . .
O1 Gd4 O5 133.4(3) . .
O6 Gd4 O5 71.3(3) . .
O1 Gd4 O4 70.7(4) . .
O6 Gd4 O4 140.3(4) . .
O5 Gd4 O4 146.1(4) . .
O1 Gd4 O3 72.2(3) . .
O6 Gd4 O3 132.9(3) . .
O5 Gd4 O3 89.6(3) . .
O4 Gd4 O3 75.0(3) . .
O1 Gd4 O7 146.9(3) . .
O6 Gd4 O7 74.9(3) . .
O5 Gd4 O7 69.8(3) . .
O4 Gd4 O7 102.3(3) . .
O3 Gd4 O7 138.8(3) . .
O1 Gd4 O16 80.9(3) . .
O6 Gd4 O16 66.4(4) . .
O5 Gd4 O16 124.7(3) . .
O4 Gd4 O16 76.2(3) . .
O3 Gd4 O16 145.6(3) . .
O7 Gd4 O16 66.1(3) . .
O1 Gd4 O25 125.7(3) . .
O6 Gd4 O25 144.1(4) . .
O5 Gd4 O25 81.0(3) . .
O4 Gd4 O25 65.3(4) . .
O3 Gd4 O25 67.2(3) . .
O7 Gd4 O25 74.4(3) . .
O16 Gd4 O25 116.0(3) . .
O1 Gd4 Gd5 111.2(2) . .
O6 Gd4 Gd5 40.4(2) . .
O5 Gd4 Gd5 81.9(2) . .
O4 Gd4 Gd5 114.2(2) . .
O3 Gd4 Gd5 170.8(2) . .
O7 Gd4 Gd5 40.6(2) . .
O16 Gd4 Gd5 42.8(2) . .
O25 Gd4 Gd5 114.7(2) . .
O1 Gd4 Gd2 82.2(3) . .
O6 Gd4 Gd2 171.7(3) . .
O5 Gd4 Gd2 111.8(2) . .
O4 Gd4 Gd2 39.3(3) . .
O3 Gd4 Gd2 41.2(2) . .
O7 Gd4 Gd2 113.4(2) . .
O16 Gd4 Gd2 115.3(2) . .
O25 Gd4 Gd2 43.5(2) . .
Gd5 Gd4 Gd2 146.35(3) . .
O1 Gd4 Gd1 37.4(2) . .
O6 Gd4 Gd1 108.2(3) . .
O5 Gd4 Gd1 107.8(2) . .
O4 Gd4 Gd1 77.5(2) . .
O3 Gd4 Gd1 36.7(2) . .
O7 Gd4 Gd1 175.5(3) . .
O16 Gd4 Gd1 118.0(2) . .
O25 Gd4 Gd1 101.5(2) . .
Gd5 Gd4 Gd1 143.65(3) . .
Gd2 Gd4 Gd1 63.57(2) . .
O1 Gd4 Gd6 108.8(2) . .
O6 Gd4 Gd6 36.4(3) . .
O5 Gd4 Gd6 36.4(2) . .
O4 Gd4 Gd6 176.6(3) . .
O3 Gd4 Gd6 108.2(2) . .
O7 Gd4 Gd6 76.2(2) . .
O16 Gd4 Gd6 100.3(2) . .
O25 Gd4 Gd6 116.9(2) . .
Gd5 Gd4 Gd6 62.66(2) . .
Gd2 Gd4 Gd6 144.10(3) . .
Gd1 Gd4 Gd6 104.20(2) . .
O19 Gd5 O7 145.8(4) 3_756 .
O19 Gd5 O20 82.5(5) 3_756 .
O7 Gd5 O20 95.2(5) . .
O19 Gd5 O6 87.4(4) 3_756 .
O7 Gd5 O6 76.7(3) . .
O20 Gd5 O6 148.3(4) . .
O19 Gd5 O17 122.1(4) 3_756 .
O7 Gd5 O17 88.7(4) . .
O20 Gd5 O17 71.7(5) . .
O6 Gd5 O17 137.4(4) . .
O19 Gd5 O8 76.9(4) 3_756 .
O7 Gd5 O8 69.3(3) . .
O20 Gd5 O8 77.6(4) . .
O6 Gd5 O8 70.9(3) . .
O17 Gd5 O8 140.3(4) . .
O19 Gd5 O18 71.3(4) 3_756 .
O7 Gd5 O18 138.8(4) . .
O20 Gd5 O18 111.4(5) . .
O6 Gd5 O18 93.4(4) . .
O17 Gd5 O18 71.7(4) . .
O8 Gd5 O18 145.1(4) . .
O19 Gd5 O16 132.9(4) 3_756 .
O7 Gd5 O16 67.8(3) . .
O20 Gd5 O16 138.3(4) . .
O6 Gd5 O16 67.1(3) . .
O17 Gd5 O16 70.3(4) . .
O8 Gd5 O16 125.0(3) . .
O18 Gd5 O16 71.5(4) . .
O19 Gd5 Gd4 128.1(3) 3_756 .
O7 Gd5 Gd4 42.3(2) . .
O20 Gd5 Gd4 137.3(4) . .
O6 Gd5 Gd4 40.8(3) . .
O17 Gd5 Gd4 104.5(3) . .
O8 Gd5 Gd4 81.5(2) . .
O18 Gd5 Gd4 107.1(3) . .
O16 Gd5 Gd4 43.4(2) . .
O19 Gd5 Gd7 111.9(3) 3_756 .
O7 Gd5 Gd7 35.2(2) . .
O20 Gd5 Gd7 79.4(4) . .
O6 Gd5 Gd7 76.7(3) . .
O17 Gd5 Gd7 112.9(3) . .
O8 Gd5 Gd7 35.1(2) . .
O18 Gd5 Gd7 169.2(3) . .
O16 Gd5 Gd7 100.3(2) . .
Gd4 Gd5 Gd7 62.59(2) . .
O19 Gd5 Gd6 73.2(3) 3_756 .
O7 Gd5 Gd6 76.4(2) . .
O20 Gd5 Gd6 112.8(3) . .
O6 Gd5 Gd6 35.7(3) . .
O17 Gd5 Gd6 164.7(3) . .
O8 Gd5 Gd6 36.5(2) . .
O18 Gd5 Gd6 117.5(3) . .
O16 Gd5 Gd6 100.2(2) . .
Gd4 Gd5 Gd6 61.849(19) . .
Gd7 Gd5 Gd6 55.88(2) . .
O9 Gd6 O36 70.7(3) . 3_756
O9 Gd6 O5 92.6(3) . .
O36 Gd6 O5 139.3(3) 3_756 .
O9 Gd6 O6 136.4(3) . .
O36 Gd6 O6 145.3(4) 3_756 .
O5 Gd6 O6 70.7(3) . .
O9 Gd6 O9 72.3(3) . 3_756
O36 Gd6 O9 75.0(3) 3_756 3_756
O5 Gd6 O9 136.2(3) . 3_756
O6 Gd6 O9 92.1(3) . 3_756
O9 Gd6 O8 145.2(3) . .
O36 Gd6 O8 98.2(3) 3_756 .
O5 Gd6 O8 74.4(3) . .
O6 Gd6 O8 70.1(3) . .
O9 Gd6 O8 138.2(3) 3_756 .
O9 Gd6 O30 79.3(3) . .
O36 Gd6 O30 74.6(3) 3_756 .
O5 Gd6 O30 65.7(3) . .
O6 Gd6 O30 124.2(3) . .
O9 Gd6 O30 143.8(3) 3_756 .
O8 Gd6 O30 65.9(3) . .
O9 Gd6 O34 125.1(3) . 3_756
O36 Gd6 O34 65.7(3) 3_756 3_756
O5 Gd6 O34 142.3(3) . 3_756
O6 Gd6 O34 79.6(3) . 3_756
O9 Gd6 O34 65.7(3) 3_756 3_756
O8 Gd6 O34 73.9(3) . 3_756
O30 Gd6 O34 117.4(3) . 3_756
O9 Gd6 Cl1 67.6(2) . .
O36 Gd6 Cl1 130.21(19) 3_756 .
O5 Gd6 Cl1 68.8(2) . .
O6 Gd6 Cl1 68.8(3) . .
O9 Gd6 Cl1 67.44(19) 3_756 .
O8 Gd6 Cl1 131.6(2) . .
O30 Gd6 Cl1 121.3(2) . .
O34 Gd6 Cl1 121.3(2) 3_756 .
O9 Gd6 Gd8 82.3(2) . 3_756
O36 Gd6 Gd8 39.6(2) 3_756 3_756
O5 Gd6 Gd8 174.8(2) . 3_756
O6 Gd6 Gd8 112.3(3) . 3_756
O9 Gd6 Gd8 40.94(19) 3_756 3_756
O8 Gd6 Gd8 110.5(2) . 3_756
O30 Gd6 Gd8 114.1(2) . 3_756
O34 Gd6 Gd8 42.8(2) 3_756 3_756
Cl1 Gd6 Gd8 107.97(4) . 3_756
O9 Gd6 Gd7 112.0(2) . .
O36 Gd6 Gd7 110.9(2) 3_756 .
O5 Gd6 Gd7 40.5(2) . .
O6 Gd6 Gd7 81.4(3) . .
O9 Gd6 Gd7 173.4(2) 3_756 .
O8 Gd6 Gd7 39.8(2) . .
O30 Gd6 Gd7 42.7(2) . .
O34 Gd6 Gd7 113.5(2) 3_756 .
Cl1 Gd6 Gd7 109.09(4) . .
Gd8 Gd6 Gd7 142.94(3) 3_756 .
O9 Gd6 Gd6 37.1(2) . 3_756
O36 Gd6 Gd6 76.74(19) 3_756 3_756
O5 Gd6 Gd6 112.2(2) . 3_756
O6 Gd6 Gd6 111.8(3) . 3_756
O9 Gd6 Gd6 36.8(2) 3_756 3_756
O8 Gd6 Gd6 173.4(2) . 3_756
O30 Gd6 Gd6 115.9(2) . 3_756
O34 Gd6 Gd6 100.0(2) 3_756 3_756
Cl1 Gd6 Gd6 53.58(4) . 3_756
Gd8 Gd6 Gd6 62.97(2) 3_756 3_756
Gd7 Gd6 Gd6 145.87(4) . 3_756
O8 Gd7 O7 69.9(3) . .
O8 Gd7 O26 145.5(3) . .
O7 Gd7 O26 77.2(4) . .
O8 Gd7 O27 98.1(5) . .
O7 Gd7 O27 77.1(4) . .
O26 Gd7 O27 84.3(5) . .
O8 Gd7 O5 75.7(3) . .
O7 Gd7 O5 71.0(3) . .
O26 Gd7 O5 84.0(4) . .
O27 Gd7 O5 147.7(4) . .
O8 Gd7 O29 138.6(3) . .
O7 Gd7 O29 146.3(4) . .
O26 Gd7 O29 70.5(4) . .
O27 Gd7 O29 108.0(5) . .
O5 Gd7 O29 96.2(3) . .
O8 Gd7 O28 88.0(3) . .
O7 Gd7 O28 138.6(4) . .
O26 Gd7 O28 124.8(4) . .
O27 Gd7 O28 71.7(4) . .
O5 Gd7 O28 138.2(3) . .
O29 Gd7 O28 71.1(4) . .
O8 Gd7 O30 68.6(3) . .
O7 Gd7 O30 126.8(3) . .
O26 Gd7 O30 128.2(4) . .
O27 Gd7 O30 140.3(4) . .
O5 Gd7 O30 67.6(3) . .
O29 Gd7 O30 70.8(3) . .
O28 Gd7 O30 70.6(3) . .
O8 Gd7 Gd6 41.1(2) . .
O7 Gd7 Gd6 81.7(2) . .
O26 Gd7 Gd6 124.6(3) . .
O27 Gd7 Gd6 138.8(4) . .
O5 Gd7 Gd6 40.7(2) . .
O29 Gd7 Gd6 109.2(2) . .
O28 Gd7 Gd6 104.6(2) . .
O30 Gd7 Gd6 45.1(2) . .
O8 Gd7 Gd5 36.02(19) . .
O7 Gd7 Gd5 35.0(2) . .
O26 Gd7 Gd5 112.2(3) . .
O27 Gd7 Gd5 80.7(4) . .
O5 Gd7 Gd5 76.0(2) . .
O29 Gd7 Gd5 171.2(2) . .
O28 Gd7 Gd5 111.9(3) . .
O30 Gd7 Gd5 102.0(2) . .
Gd6 Gd7 Gd5 62.18(2) . .
O8 Gd7 Gd4 75.9(2) . .
O7 Gd7 Gd4 36.7(2) . .
O26 Gd7 Gd4 71.4(3) . .
O27 Gd7 Gd4 112.3(4) . .
O5 Gd7 Gd4 35.4(2) . .
O29 Gd7 Gd4 120.1(3) . .
O28 Gd7 Gd4 163.7(3) . .
O30 Gd7 Gd4 100.8(2) . .
Gd6 Gd7 Gd4 61.51(2) . .
Gd5 Gd7 Gd4 55.28(2) . .
O31 Gd8 O36 145.8(3) . .
O31 Gd8 O35 84.3(5) . .
O36 Gd8 O35 99.7(5) . .
O31 Gd8 O9 82.9(3) . .
O36 Gd8 O9 75.8(3) . .
O35 Gd8 O9 147.7(4) . .
O31 Gd8 O36 77.6(3) . 3_756
O36 Gd8 O36 70.2(3) . 3_756
O35 Gd8 O36 78.3(4) . 3_756
O9 Gd8 O36 70.0(3) . 3_756
O31 Gd8 O32 125.9(4) . .
O36 Gd8 O32 87.1(4) . .
O35 Gd8 O32 72.7(4) . .
O9 Gd8 O32 137.6(3) . .
O36 Gd8 O32 139.3(4) 3_756 .
O31 Gd8 O33 70.5(4) . .
O36 Gd8 O33 137.4(3) . .
O35 Gd8 O33 107.3(5) . .
O9 Gd8 O33 96.1(3) . .
O36 Gd8 O33 146.7(3) 3_756 .
O32 Gd8 O33 70.9(4) . .
O31 Gd8 O34 126.8(4) . .
O36 Gd8 O34 68.3(3) . .
O35 Gd8 O34 141.3(4) . .
O9 Gd8 O34 67.5(3) . .
O36 Gd8 O34 126.0(3) 3_756 .
O32 Gd8 O34 70.1(3) . .
O33 Gd8 O34 70.0(3) . .
O31 Gd8 Gd6 123.7(2) . 3_756
O36 Gd8 Gd6 40.6(2) . 3_756
O35 Gd8 Gd6 139.8(4) . 3_756
O9 Gd8 Gd6 40.9(2) . 3_756
O36 Gd8 Gd6 80.6(2) 3_756 3_756
O32 Gd8 Gd6 103.9(3) . 3_756
O33 Gd8 Gd6 109.1(3) . 3_756
O34 Gd8 Gd6 45.4(2) . 3_756
O31 Gd8 Gd8 112.9(3) . 3_756
O36 Gd8 Gd8 36.5(2) . 3_756
O35 Gd8 Gd8 80.8(4) . 3_756
O9 Gd8 Gd8 77.20(19) . 3_756
O36 Gd8 Gd8 35.4(2) 3_756 3_756
O32 Gd8 Gd8 110.7(3) . 3_756
O33 Gd8 Gd8 171.7(3) . 3_756
O34 Gd8 Gd8 102.6(2) . 3_756
Gd6 Gd8 Gd8 62.62(2) 3_756 3_756
O31 Gd8 Gd6 71.6(2) . .
O36 Gd8 Gd6 75.6(2) . .
O35 Gd8 Gd6 112.4(3) . .
O9 Gd8 Gd6 35.3(2) . .
O36 Gd8 Gd6 35.8(2) 3_756 .
O32 Gd8 Gd6 162.5(3) . .
O33 Gd8 Gd6 120.7(3) . .
O34 Gd8 Gd6 100.4(2) . .
Gd6 Gd8 Gd6 60.93(2) 3_756 .
Gd8 Gd8 Gd6 55.844(19) 3_756 .
Gd4 O1 Gd1 106.6(4) . .
Gd4 O1 Gd3 109.5(4) . .
Gd1 O1 Gd3 98.4(3) . .
Gd1 O2 Gd3 101.8(4) . .
Gd1 O2 Gd2 110.6(4) . .
Gd3 O2 Gd2 106.2(4) . .
Gd1 O3 Gd2 110.6(4) . .
Gd1 O3 Gd4 105.8(4) . .
Gd2 O3 Gd4 97.1(3) . .
Gd2 O4 Gd3 107.8(4) . .
Gd2 O4 Gd4 99.5(4) . .
Gd3 O4 Gd4 108.7(4) . .
Gd4 O5 Gd7 109.1(3) . .
Gd4 O5 Gd6 107.3(4) . .
Gd7 O5 Gd6 98.8(4) . .
Gd5 O6 Gd4 98.8(4) . .
Gd5 O6 Gd6 109.2(4) . .
Gd4 O6 Gd6 107.5(4) . .
Gd5 O7 Gd7 109.8(4) . .
Gd5 O7 Gd4 97.1(3) . .
Gd7 O7 Gd4 107.7(4) . .
Gd7 O8 Gd5 108.9(3) . .
Gd7 O8 Gd6 99.2(3) . .
Gd5 O8 Gd6 107.2(3) . .
Gd6 O9 Gd6 106.1(3) . 3_756
Gd6 O9 Gd8 109.0(3) . .
Gd6 O9 Gd8 98.2(3) 3_756 .
C1 O10 Gd3 134.6(11) . .
C1 O10 Gd1 132.9(11) . .
Gd3 O10 Gd1 92.4(4) . .
C4 O11 Gd3 133.7(12) . .
C3 O12 Gd3 120.6(12) . .
C6 O15 Gd3 139.2(10) . .
C6 O16 Gd5 129.9(10) . .
C6 O16 Gd4 135.3(10) . .
Gd5 O16 Gd4 93.7(3) . .
C8 O17 Gd5 131.5(11) . .
C9 O18 Gd5 131.2(12) . .
C23 O19 Gd5 137.6(10) . 3_756
C1 O22 Gd2 142.6(14) . 3_756
C13 O23 Gd2 132.5(13) . .
C14 O24 Gd2 127.9(11) . .
C11 O25 Gd2 132.7(10) . .
C11 O25 Gd4 134.9(10) . .
Gd2 O25 Gd4 92.0(3) . .
C11 O26 Gd7 138.7(11) . .
C19 O28 Gd7 127.7(10) . .
C18 O29 Gd7 131.5(10) . .
C16 O30 Gd7 130.5(9) . .
C16 O30 Gd6 137.3(9) . .
Gd7 O30 Gd6 92.2(3) . .
C16 O31 Gd8 143.1(10) . .
C24 O32 Gd8 131.0(9) . .
C21 O33 Gd8 133.2(10) . .
C23 O34 Gd8 133.2(9) . .
C23 O34 Gd6 134.9(9) . 3_756
Gd8 O34 Gd6 91.8(3) . 3_756
Gd8 O36 Gd6 99.8(3) . 3_756
Gd8 O36 Gd8 108.1(3) . 3_756
Gd6 O36 Gd8 108.2(3) 3_756 3_756
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 O22 1.17(3) .
C1 O10 1.29(2) .
C1 C2 1.54(3) .
C2 C3 1.41(3) .
C2 C4 1.53(3) .
C2 C5 1.66(3) .
C3 O12 1.57(3) .
C4 O11 1.50(3) .
C6 O16 1.241(19) .
C6 O15 1.27(2) .
C6 C7 1.54(2) .
C7 C8 1.57(3) .
C7 C9 1.59(3) .
C7 C10 1.61(2) .
C8 O17 1.40(2) .
C9 O18 1.35(2) .
C11 O26 1.18(2) .
C11 O25 1.276(19) .
C11 C12 1.59(2) .
C12 C13 1.48(3) .
C12 C14 1.49(2) .
C12 C15 1.53(3) .
C13 O23 1.34(2) .
C14 O24 1.44(2) .
C16 O31 1.250(17) .
C16 O30 1.264(17) .
C16 C17 1.54(2) .
C17 C18 1.48(2) .
C17 C19 1.53(2) .
C17 C20 1.56(2) .
C18 O29 1.430(19) .
C19 O28 1.415(18) .
C21 O33 1.406(19) .
C21 C22 1.58(3) .
C22 C23 1.53(2) .
C22 C25 1.58(2) .
C22 C24 1.58(2) .
C23 O19 1.224(19) .
C23 O34 1.241(17) .
C24 O32 1.430(18) .
Cl1 Gd1 3.154(4) .
Cl1 Gd6 3.224(3) 3_756
Cl1 Gd6 3.224(3) .
Gd1 O3 2.369(10) 3_756
Gd1 O3 2.369(10) .
Gd1 O2 2.368(10) 3_756
Gd1 O2 2.369(10) .
Gd1 O1 2.421(9) 3_756
Gd1 O1 2.421(9) .
Gd1 O10 2.639(11) 3_756
Gd1 O10 2.639(11) .
Gd1 Gd3 3.6825(9) 3_756
Gd1 Gd3 3.6826(9) .
Gd1 Gd4 3.8183(10) .
Gd2 O22 2.311(13) 3_756
Gd2 O4 2.321(11) .
Gd2 O2 2.395(10) .
Gd2 O3 2.396(9) .
Gd2 O24 2.397(13) .
Gd2 O23 2.426(14) .
Gd2 O25 2.489(10) .
Gd2 Gd4 3.6111(12) .
Gd2 Gd3 3.8159(14) .
Gd3 O13 2.253(9) .
Gd3 O15 2.371(10) .
Gd3 O2 2.377(11) .
Gd3 O4 2.401(11) .
Gd3 O14 2.419(15) .
Gd3 O11 2.435(13) .
Gd3 O12 2.441(14) .
Gd3 O1 2.443(10) .
Gd3 O10 2.460(11) .
Gd3 Gd4 3.9078(12) .
Gd4 O1 2.342(10) .
Gd4 O6 2.383(11) .
Gd4 O5 2.390(9) .
Gd4 O4 2.409(10) .
Gd4 O3 2.420(9) .
Gd4 O7 2.446(9) .
Gd4 O16 2.486(9) .
Gd4 O25 2.531(11) .
Gd4 Gd5 3.6072(11) .
Gd4 Gd6 3.8597(10) .
Gd5 O19 2.311(11) 3_756
Gd5 O7 2.364(11) .
Gd5 O20 2.366(14) .
Gd5 O6 2.367(10) .
Gd5 O17 2.400(10) .
Gd5 O8 2.411(8) .
Gd5 O18 2.444(11) .
Gd5 O16 2.457(10) .
Gd5 Gd7 3.8795(12) .
Gd5 Gd6 3.8885(10) .
Gd6 O9 2.386(9) .
Gd6 O36 2.400(8) 3_756
Gd6 O5 2.402(10) .
Gd6 O6 2.402(11) .
Gd6 O9 2.403(9) 3_756
Gd6 O8 2.422(8) .
Gd6 O30 2.580(10) .
Gd6 O34 2.590(9) 3_756
Gd6 Gd8 3.6354(10) 3_756
Gd6 Gd7 3.6399(11) .
Gd6 Gd6 3.8278(14) 3_756
Gd7 O8 2.359(10) .
Gd7 O7 2.378(10) .
Gd7 O26 2.378(11) .
Gd7 O27 2.390(15) .
Gd7 O5 2.392(9) .
Gd7 O29 2.415(11) .
Gd7 O28 2.445(10) .
Gd7 O30 2.472(9) .
Gd8 O31 2.320(10) .
Gd8 O36 2.353(9) .
Gd8 O35 2.378(13) .
Gd8 O9 2.406(8) .
Gd8 O36 2.417(9) 3_756
Gd8 O32 2.431(10) .
Gd8 O33 2.456(11) .
Gd8 O34 2.471(9) .
Gd8 Gd6 3.6355(10) 3_756
Gd8 Gd8 3.8621(16) 3_756
O9 Gd6 2.403(9) 3_756
O19 Gd5 2.311(11) 3_756
O22 Gd2 2.311(13) 3_756
O34 Gd6 2.590(9) 3_756
O36 Gd6 2.400(8) 3_756
O36 Gd8 2.417(9) 3_756
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.046 -0.009 -0.016 8668 5205 ' '
